     • date post

05-Jun-2018
• Category

## Documents

• view

228

3

Embed Size (px)

### Transcript of Plasticity and Deformation Process - Metalurji Ve Malzeme ...· deformation theory of plasticity...

• Plasticity and Deformation Process

Stress-strain relations in deformation theory

• The fundamental problem in the solution of a plasticity problem is to determine how stresses and strains can be found for a specified state of loading on a body.

There are two theories to describe the relation between stresses and strains:

Deformation or total strain theory:

Total strains are directly related to the total stresses by the secant modulus which is a function of the stress levelThe strains on an object depend on the final state of stress, they are independent of stress history

Flow or incremental strain theory:Increments of plastic strain P are related to increments of plastic stress P by the tangent modulus which is a function of the stress level

• The strains are separated into an elastic component e and a plastic component P in both theories.

The plastic component is represented by a complex equation as will be derived next

Both deformation and incremental theories are based on the assumption that elastic deformation is compressible and plastic deformation is incompressible

• The compressible nature of elastic deformation is obvious from the fact that Poissons ratio for ordinary isotropic materials is much less than one-half (0-0.35)

The incompressibilty of plastic deformation is not obvious

Experiments on materials subjected to very high hydrostatic pressures show that the density and volume do not significantly change under extremely high pressures.

Recall the dilatation or volumetric strain of materials under hydrostatic stress:

= + + = 1 2

In which is the total strain under uniaxial stress and is the Poissons ratio for total strains

Dilatation can be regarded as the sum of an elastic dilatation and a plastic dilatation

= 1 2 = 1 2

• = + = 1 2 = 1 2 + 1 2

Dividing both sides by and substituting for gives:

1 2 =

1 2 +

1 2

2 =

2 2 +

2

So

=

Furthermore the strains can be expressed in terms of the moduli:

=

=

Finally

=

Or

=1

2

1

2

• Since materials are incompressible during plastic deformation, the Poissons ratio changes from the elastic value to the incompressible value in a very gradual way as the stress is increased above the yield stress

= for

= =1

2

1

2 for >

=1

2for

• The stress-strain relations are expressed by Hencky et al. according to the deformation theory

Strains are separated into elastic and plastic strains:

= +

= +

The elastic strains are obtained from the Hookes law

=

1

+

=

1

+

=

1

+

=

=

=

Where the mechanical properties E and G are the normal elastic modulus and shear modulus

• To obtain the plastic moduli we need to consider the stress-strain diagram in terms of the normal stress and the plastic strain

The plastic modulus at any stress above the yield stress is the secant modulus at that point

=

1

+

=

1

+

=

1

+

=

=

=

Where is the plastic Poissons ratio (1/2) and is the plastic shear modulus:

=

2 1 + =

3

• The elastic and plastic strains sum to the total strains as

1

=1

+

1

= +

1 + 1

The stress-strain behavior is divided into three regions: elastic, elastic-plastic and plastic

Only the elastic-plastic region is considered in the deformation theory as a material nonlinearity

• The modulus is expressed as a function of the stresses using various material models.

The problem-solving is not straight forward because the secant modulus depends on the stress and an iteration procedure is essential.

Hencky used the von Mises yield criterion and the distortional energy concept to derive the stress-strain relations

The combination of the yield criterion, the stress-strain relations, and the material model is the complete deformation theory of plasticity

Deformation theory helps us predict the stresses and strains at a point on the stress-strain curve but does not enable consideration of the path taken to get there.

Because of that, loading and unloading can not be evaluated with the same material model using deformation theory and should be considered as separate events.

Another limitation of deformation theory is that all stresses in a multiaxial stress state must be applied in proportion to one another because deformation theory is not capable of distinguishing between types of loading.

Also hardening is considered isotropic because the secant modulus is used instead of the tangent modulus.

These restrictions are valid for some plasticity problems and the theory is not generally applicable.

But it is applicable to most practical problems in metal forming and quite useful. Some problems that are easily solved with deformation theory are difficult to solve with incremental theory because of the excessively complex computation methods.

• The basis for the deformation theory of plasticity is the stress-strain relations and the associated stress and strain intensities for multiaxial stress states.

The stress intensity or the effective stress for an elastic material is expressed as

=2

2

2+

2+

2 + 6 2 +

2 + 2

And the effective strain as

=2

2 1 +

2+

2+

2 +3

2

2 + 2 +

2

And =

The three dimensional elastic stress-strain relations for an isotropic material in terms of Youngs modulus, and Poissons ratio are:

=

1 + 1 21 + +

=

1 + 1 21 + +

=

1 + 1 21 + +

=

2 1 +

=

2 1 +

=

2 1 +

• Partitioning of the strains into elastic and plastic components helps us understand the deformation theory. In practice it is more convenient to determine the strains from a state of multiaxial stress in a single form that applies to all three deformation regions

These three dimensional total stress-strain relatios for an isotropic material in terms of Youngs secant modulus and a continuously variable Poissons ratio are similarly:

=

1 + 1 21 + +

=

1 + 1 21 + +

=

1 + 1 21 + +

=2 1 +

=

=2 1 +

=

=2 1 +

=

Where

=1

2

1

2

And

=

2 1 +

• Most deformation processes involving thin plates of material are approximated to the plane stress conditions

Plane stress is a state of stress in which the normal stress , and the shear stresses , directed

perpendicular to the x-y plane are assumed to be zero

The geometry of the body is that of a plate with one dimension much smaller than the others. The loads are applied uniformly over the thickness of the plate and act in the plane of the plate as shown.

The plane stress condition is the simplest form of behavior for continuum structures and represents situations frequently encountered in practice

• Under plane stress conditions = 0, = = 0 and =

1 +

So the effective strain for a state of plane stress is

=2

2 1 21 + 2

2 + 2 + 1 4 + 2 +

3

41 2

2

And the effective stress is

=2

2

2+

2+

2 + 6 2

Example A thin disk of aluminum is stressed under plane stress conditions. Determine the effective stress and strain resulting from the load if the normal stresses in the x and y direction are 70 MPa and 40 MPa, and the shearing stress on the plane is 30 MPa. EAl= 70 GPa

• Deformation theory is workable only if and are expressed as a function of the multiaxial stress stateRecall that

=1

2

1

2

The should be expressed as a function of the multiaxial stress state

The general effective stress equation is

=2

2

2+

2+

2 + 6 2 +

2 + 2

And the general effective strain

=2

2 1 +

2+

2+

2 +3

2

2 + 2 +

2

And

=

The equalization of the - curve to the uniaxial curve when the stresses applied to the material

are reduced to uniaxial state of stress enables us to determine the empirically and solve the deformation theory problem:

=2

2 2 + 2 =

And

=2

2 1 + 2 1 + 2 + 2 + 2 1 2 =

Hence

=

• Relating the material properties , for deformation under a multiaxial stress state to the properties determined in the usual uniaxial mechanical characterization test is important especially for materials with nonlinear stress-strain behavior as their properties are a nonlinear function of all the multiaxial stresses that act.

The curve obtained from the uniaxial test is the same as the - curve which represents all multiaxial

stress. This remarkable identity makes the uniaxial stress-strain curve the universal stress-strain curve

• To obtain the secant modulus form a uniaxial stress-strain curve, the curve should be considered as a set of points each of which is a stress and corresponding strain that are obtained during a measurement.

Enter the stress-strain curve at a specific value of corresponding to the given multiaxial stress state